#------------------------------------------------------------------------------
#$Date: 2016-03-23 23:39:14 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179510 $
#$URL: svn://www.crystallography.net/cod/cif/4/34/07/4340758.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4340758
loop_
_publ_author_name
'Lin, Jian'
'Diefenbach, Kariem'
'Kikugawa, Naoki'
'Baumbach, Ryan E.'
'Albrecht-Schmitt, Thomas E'
_publ_section_title
;
 Dimensional and coordination number reductions in a large family of
 lanthanide tellurite sulfates.
;
_journal_issue                   16
_journal_name_full               'Inorganic chemistry'
_journal_page_first              8555
_journal_page_last               8564
_journal_paper_doi               10.1021/ic501163x
_journal_volume                  53
_journal_year                    2014
_chemical_formula_moiety         Ho2TeO3(SO4)2(H2O)2
_chemical_formula_sum            'Ho2 O13 S2 Te'
_chemical_formula_weight         729.58
_chemical_melting_point          ?
_chemical_name_common            'Holmium tellurite sulfate'
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.7190(10)
_cell_angle_beta                 101.505(2)
_cell_angle_gamma                103.809(2)
_cell_formula_units_Z            2
_cell_length_a                   5.3462(7)
_cell_length_b                   8.2012(11)
_cell_length_c                   12.3034(17)
_cell_measurement_reflns_used    2338
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      27.50
_cell_measurement_theta_min      1.69
_cell_volume                     512.30(12)
_computing_cell_refinement       'smart saint'
_computing_data_collection       smart
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXP-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELXCIF-97 (Sheldrick, 2000)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean 0
_diffrn_measured_fraction_theta_full 0.982
_diffrn_measured_fraction_theta_max 0.982
_diffrn_measurement_device_type  'BRUKER apex II'
_diffrn_measurement_method       '0.5 wide w/ exposures'
_diffrn_radiation_monochromator  'Quazar optics'
_diffrn_radiation_source         'Imus microfocused'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0000
_diffrn_reflns_av_sigmaI/netI    0.0510
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            2297
_diffrn_reflns_theta_full        27.50
_diffrn_reflns_theta_max         27.50
_diffrn_reflns_theta_min         1.69
_exptl_absorpt_coefficient_mu    18.601
_exptl_absorpt_correction_T_max  0.928
_exptl_absorpt_correction_T_min  0.894
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   SHELTXPREP
_exptl_crystal_colour            pink
_exptl_crystal_density_diffrn    4.730
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Columnar
_exptl_crystal_F_000             644
_exptl_crystal_size_max          0.019
_exptl_crystal_size_mid          0.005
_exptl_crystal_size_min          0.004
_refine_diff_density_max         1.736
_refine_diff_density_min         -1.951
_refine_diff_density_rms         0.309
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.041
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     163
_refine_ls_number_reflns         2297
_refine_ls_number_restraints     6
_refine_ls_restrained_S_all      1.040
_refine_ls_R_factor_all          0.0370
_refine_ls_R_factor_gt           0.0297
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0198P)²+4.2071P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0681
_refine_ls_wR_factor_ref         0.0707
_reflns_number_gt                2020
_reflns_number_total             2297
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic501163x_si_002.cif
_cod_data_source_block           Ho3
_cod_depositor_comments
;
The following automatic conversions were performed:

'_chemical_melting_point' value 'N/A' was changed to '?' - the value
is undefined or not given.

'_symmetry_cell_setting' value
'Triclinic' changed to 'triclinic' according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 

 Adding full bibliography for 4340748--4340769.cif.

The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'N/A' was changed to '?' - the
value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_original_sg_symbol_H-M      P-1
_cod_database_code               4340758
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ho1 Ho 0.15125(7) 0.02623(4) 0.37154(3) 0.00906(11) Uani 1 1 d .
Ho2 Ho 1.21771(7) 0.35609(5) 0.17188(3) 0.00912(11) Uani 1 1 d .
Te1 Te 0.78592(10) 0.29768(7) 0.39543(4) 0.01190(13) Uani 1 1 d .
S1 S 0.5496(4) -0.2712(2) 0.36422(16) 0.0094(4) Uani 1 1 d .
S2 S 1.3997(4) 0.7397(2) 0.02630(16) 0.0098(4) Uani 1 1 d .
O1 O 0.9845(11) 0.2456(7) 0.2986(5) 0.0125(12) Uani 1 1 d .
O2 O 0.8096(11) 0.0974(7) 0.4628(5) 0.0110(11) Uani 1 1 d .
O3 O 0.4702(10) 0.2124(7) 0.3005(4) 0.0087(11) Uani 1 1 d .
O4 O 0.3854(11) 0.2564(7) 0.5121(4) 0.0140(12) Uani 1 1 d .
O5 O 0.3387(11) -0.1855(7) 0.3249(5) 0.0124(12) Uani 1 1 d .
O6 O -0.2147(11) -0.1961(7) 0.3219(5) 0.0149(12) Uani 1 1 d .
O7 O 0.4548(11) -0.4514(7) 0.3269(5) 0.0141(12) Uani 1 1 d U
O8 O 0.9388(12) 0.5456(8) 0.1925(5) 0.0205(13) Uani 1 1 d .
O9 O 0.0642(12) 0.0126(8) 0.1640(5) 0.0176(13) Uani 1 1 d .
O10 O 1.4181(12) 0.5886(8) 0.0899(5) 0.0193(13) Uani 1 1 d .
O11 O 0.8807(11) 0.2747(9) 0.0240(5) 0.0217(14) Uani 1 1 d .
O12 O 1.4492(13) 0.2575(8) 0.0621(5) 0.0224(15) Uani 1 1 d .
O13 O 1.5018(13) 0.8913(8) 0.0988(5) 0.0216(14) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ho Ho -0.2175 4.6783 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Ho1 O6 82.7(2) 2_656 .
O2 Ho1 O1 136.24(19) 2_656 1_455
O6 Ho1 O1 100.9(2) . 1_455
O2 Ho1 O5 81.50(19) 2_656 .
O6 Ho1 O5 78.6(2) . .
O1 Ho1 O5 142.20(19) 1_455 .
O2 Ho1 O3 129.13(19) 2_656 .
O6 Ho1 O3 143.0(2) . .
O1 Ho1 O3 70.45(18) 1_455 .
O5 Ho1 O3 87.21(19) . .
O2 Ho1 O4 74.76(19) 2_656 .
O6 Ho1 O4 144.89(19) . .
O1 Ho1 O4 78.8(2) 1_455 .
O5 Ho1 O4 122.90(19) . .
O3 Ho1 O4 70.57(19) . .
O2 Ho1 O9 151.9(2) 2_656 .
O6 Ho1 O9 76.9(2) . .
O1 Ho1 O9 67.6(2) 1_455 .
O5 Ho1 O9 75.7(2) . .
O3 Ho1 O9 66.46(19) . .
O4 Ho1 O9 131.94(19) . .
O2 Ho1 O2 74.3(2) 2_656 1_455
O6 Ho1 O2 74.44(19) . 1_455
O1 Ho1 O2 65.06(18) 1_455 1_455
O5 Ho1 O2 145.68(19) . 1_455
O3 Ho1 O2 126.99(19) . 1_455
O4 Ho1 O2 73.78(18) . 1_455
O9 Ho1 O2 117.38(19) . 1_455
O2 Ho1 Te1 104.61(14) 2_656 1_455
O6 Ho1 Te1 92.44(15) . 1_455
O1 Ho1 Te1 32.24(13) 1_455 1_455
O5 Ho1 Te1 168.59(14) . 1_455
O3 Ho1 Te1 95.95(13) . 1_455
O4 Ho1 Te1 68.38(14) . 1_455
O9 Ho1 Te1 95.45(14) . 1_455
O2 Ho1 Te1 33.61(13) 1_455 1_455
O2 Ho1 Te1 102.03(14) 2_656 .
O6 Ho1 Te1 163.03(14) . .
O1 Ho1 Te1 87.11(14) 1_455 .
O5 Ho1 Te1 85.87(14) . .
O3 Ho1 Te1 27.40(13) . .
O4 Ho1 Te1 51.12(13) . .
O9 Ho1 Te1 92.69(14) . .
O2 Ho1 Te1 122.51(13) 1_455 .
Te1 Ho1 Te1 101.97(2) 1_455 .
O2 Ho1 Ho2 159.54(14) 2_656 1_455
O6 Ho1 Ho2 115.56(15) . 1_455
O1 Ho1 Ho2 35.73(12) 1_455 1_455
O5 Ho1 Ho2 110.09(14) . 1_455
O3 Ho1 Ho2 39.10(13) . 1_455
O4 Ho1 Ho2 84.78(13) . 1_455
O9 Ho1 Ho2 48.01(14) . 1_455
O2 Ho1 Ho2 100.61(13) 1_455 1_455
Te1 Ho1 Ho2 67.199(14) 1_455 1_455
Te1 Ho1 Ho2 63.427(12) . 1_455
O2 Ho1 Ho1 39.15(14) 2_656 2_556
O6 Ho1 Ho1 75.38(14) . 2_556
O1 Ho1 Ho1 98.97(13) 1_455 2_556
O5 Ho1 Ho1 116.94(14) . 2_556
O3 Ho1 Ho1 140.56(14) . 2_556
O4 Ho1 Ho1 70.10(13) . 2_556
O9 Ho1 Ho1 146.04(14) . 2_556
O2 Ho1 Ho1 35.20(13) 1_455 2_556
Te1 Ho1 Ho1 66.730(14) 1_455 2_556
Te1 Ho1 Ho1 118.496(18) . 2_556
Ho2 Ho1 Ho1 132.969(17) 1_455 2_556
O1 Ho2 O11 95.4(2) . .
O1 Ho2 O12 135.0(2) . .
O11 Ho2 O12 83.8(2) . .
O1 Ho2 O10 149.5(2) . .
O11 Ho2 O10 93.5(2) . .
O12 Ho2 O10 75.0(2) . .
O1 Ho2 O3 70.30(19) . 1_655
O11 Ho2 O3 134.6(2) . 1_655
O12 Ho2 O3 78.6(2) . 1_655
O10 Ho2 O3 121.1(2) . 1_655
O1 Ho2 O7 81.7(2) . 1_665
O11 Ho2 O7 151.0(2) . 1_665
O12 Ho2 O7 118.5(2) . 1_665
O10 Ho2 O7 76.5(2) . 1_665
O3 Ho2 O7 71.60(19) 1_655 1_665
O1 Ho2 O8 74.3(2) . .
O11 Ho2 O8 77.3(2) . .
O12 Ho2 O8 146.9(2) . .
O10 Ho2 O8 79.2(2) . .
O3 Ho2 O8 133.3(2) 1_655 .
O7 Ho2 O8 74.1(2) 1_665 .
O1 Ho2 O9 64.1(2) . 1_655
O11 Ho2 O9 73.1(2) . 1_655
O12 Ho2 O9 72.9(2) . 1_655
O10 Ho2 O9 146.2(2) . 1_655
O3 Ho2 O9 61.83(18) 1_655 1_655
O7 Ho2 O9 128.79(18) 1_665 1_655
O8 Ho2 O9 125.29(19) . 1_655
O1 Ho2 Ho1 36.73(14) . 1_655
O11 Ho2 Ho1 107.76(17) . 1_655
O12 Ho2 Ho1 100.83(15) . 1_655
O10 Ho2 Ho1 157.94(17) . 1_655
O3 Ho2 Ho1 37.94(12) 1_655 1_655
O7 Ho2 Ho1 87.09(13) 1_665 1_655
O8 Ho2 Ho1 110.70(15) . 1_655
O9 Ho2 Ho1 42.77(12) 1_655 1_655
O3 Te1 O1 94.5(3) . .
O3 Te1 O2 96.4(2) . .
O1 Te1 O2 88.2(2) . .
O3 Te1 Ho1 105.69(17) . 1_655
O1 Te1 Ho1 41.59(17) . 1_655
O2 Te1 Ho1 47.75(16) . 1_655
O3 Te1 Ho1 35.82(16) . .
O1 Te1 Ho1 115.85(19) . .
O2 Te1 Ho1 69.61(17) . .
Ho1 Te1 Ho1 101.97(2) 1_655 .
O6 S1 O5 110.9(4) 1_655 .
O6 S1 O7 109.9(3) 1_655 .
O5 S1 O7 109.2(3) . .
O6 S1 O4 109.5(3) 1_655 2_656
O5 S1 O4 108.8(3) . 2_656
O7 S1 O4 108.6(3) . 2_656
O13 S2 O12 110.6(4) . 2_865
O13 S2 O11 109.4(4) . 2_765
O12 S2 O11 109.7(4) 2_865 2_765
O13 S2 O10 110.7(4) . .
O12 S2 O10 108.1(4) 2_865 .
O11 S2 O10 108.2(4) 2_765 .
Te1 O1 Ho2 142.7(3) . .
Te1 O1 Ho1 106.2(2) . 1_655
Ho2 O1 Ho1 107.5(2) . 1_655
Te1 O2 Ho1 144.2(3) . 2_656
Te1 O2 Ho1 98.6(2) . 1_655
Ho1 O2 Ho1 105.7(2) 2_656 1_655
Te1 O3 Ho1 116.8(3) . .
Te1 O3 Ho2 128.6(3) . 1_455
Ho1 O3 Ho2 102.96(19) . 1_455
S1 O4 Ho1 134.5(3) 2_656 .
S1 O5 Ho1 143.5(3) . .
S1 O6 Ho1 137.6(4) 1_455 .
S1 O7 Ho2 143.8(3) . 1_445
Ho1 O9 Ho2 89.22(19) . 1_455
S2 O10 Ho2 149.7(4) . .
S2 O11 Ho2 148.4(4) 2_765 .
S2 O12 Ho2 157.0(4) 2_865 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ho1 O2 2.282(5) 2_656
Ho1 O6 2.306(6) .
Ho1 O1 2.308(6) 1_455
Ho1 O5 2.320(6) .
Ho1 O3 2.321(5) .
Ho1 O4 2.459(6) .
Ho1 O9 2.499(6) .
Ho1 O2 2.500(5) 1_455
Ho1 Te1 3.3385(7) 1_455
Ho1 Te1 3.5405(7) .
Ho1 Ho2 3.6790(6) 1_455
Ho1 Ho1 3.8123(8) 2_556
Ho2 O1 2.253(5) .
Ho2 O11 2.256(6) .
Ho2 O12 2.265(6) .
Ho2 O10 2.304(6) .
Ho2 O3 2.381(5) 1_655
Ho2 O7 2.396(6) 1_665
Ho2 O8 2.439(6) .
Ho2 O9 2.735(6) 1_655
Ho2 Ho1 3.6790(6) 1_655
Te1 O3 1.825(5) .
Te1 O1 1.854(5) .
Te1 O2 1.869(6) .
Te1 Ho1 3.3385(7) 1_655
S1 O6 1.462(6) 1_655
S1 O5 1.473(6) .
S1 O7 1.478(6) .
S1 O4 1.488(6) 2_656
S2 O13 1.447(6) .
S2 O12 1.475(6) 2_865
S2 O11 1.479(6) 2_765
S2 O10 1.486(6) .
O1 Ho1 2.308(6) 1_655
O2 Ho1 2.282(5) 2_656
O2 Ho1 2.500(5) 1_655
O3 Ho2 2.381(5) 1_455
O4 S1 1.488(6) 2_656
O6 S1 1.462(5) 1_455
O7 Ho2 2.396(6) 1_445
O9 Ho2 2.735(6) 1_455
O11 S2 1.479(6) 2_765
O12 S2 1.475(6) 2_865
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O2 Ho1 Te1 O3 172.3(3) 2_656 .
O6 Ho1 Te1 O3 67.8(6) . .
O1 Ho1 Te1 O3 -50.9(3) 1_455 .
O5 Ho1 Te1 O3 91.9(3) . .
O4 Ho1 Te1 O3 -128.8(3) . .
O9 Ho1 Te1 O3 16.4(3) . .
O2 Ho1 Te1 O3 -108.7(3) 1_455 .
Te1 Ho1 Te1 O3 -79.7(3) 1_455 .
Ho2 Ho1 Te1 O3 -23.0(3) 1_455 .
Ho1 Ho1 Te1 O3 -149.6(3) 2_556 .
O2 Ho1 Te1 O1 113.7(2) 2_656 .
O6 Ho1 Te1 O1 9.2(6) . .
O1 Ho1 Te1 O1 -109.5(3) 1_455 .
O5 Ho1 Te1 O1 33.3(2) . .
O3 Ho1 Te1 O1 -58.6(3) . .
O4 Ho1 Te1 O1 172.6(3) . .
O9 Ho1 Te1 O1 -42.2(2) . .
O2 Ho1 Te1 O1 -167.3(2) 1_455 .
Te1 Ho1 Te1 O1 -138.31(19) 1_455 .
Ho2 Ho1 Te1 O1 -81.61(19) 1_455 .
Ho1 Ho1 Te1 O1 151.83(19) 2_556 .
O2 Ho1 Te1 O2 36.3(3) 2_656 .
O6 Ho1 Te1 O2 -68.2(5) . .
O1 Ho1 Te1 O2 173.1(2) 1_455 .
O5 Ho1 Te1 O2 -44.1(2) . .
O3 Ho1 Te1 O2 -136.0(3) . .
O4 Ho1 Te1 O2 95.2(2) . .
O9 Ho1 Te1 O2 -119.6(2) . .
O2 Ho1 Te1 O2 115.3(3) 1_455 .
Te1 Ho1 Te1 O2 144.29(18) 1_455 .
Ho2 Ho1 Te1 O2 -159.00(18) 1_455 .
Ho1 Ho1 Te1 O2 74.44(18) 2_556 .
O2 Ho1 Te1 Ho1 72.01(14) 2_656 1_655
O6 Ho1 Te1 Ho1 -32.5(5) . 1_655
O1 Ho1 Te1 Ho1 -151.22(14) 1_455 1_655
O5 Ho1 Te1 Ho1 -8.38(14) . 1_655
O3 Ho1 Te1 Ho1 -100.3(3) . 1_655
O4 Ho1 Te1 Ho1 130.89(17) . 1_655
O9 Ho1 Te1 Ho1 -83.85(14) . 1_655
O2 Ho1 Te1 Ho1 150.98(15) 1_455 1_655
Te1 Ho1 Te1 Ho1 180.0 1_455 1_655
Ho2 Ho1 Te1 Ho1 -123.293(17) 1_455 1_655
Ho1 Ho1 Te1 Ho1 110.149(18) 2_556 1_655
O3 Te1 O1 Ho2 97.4(5) . .
O2 Te1 O1 Ho2 -166.3(5) . .
Ho1 Te1 O1 Ho2 -154.0(7) 1_655 .
Ho1 Te1 O1 Ho2 127.5(4) . .
O3 Te1 O1 Ho1 -108.6(3) . 1_655
O2 Te1 O1 Ho1 -12.3(3) . 1_655
Ho1 Te1 O1 Ho1 -78.5(2) . 1_655
O11 Ho2 O1 Te1 -93.5(5) . .
O12 Ho2 O1 Te1 179.9(4) . .
O10 Ho2 O1 Te1 12.7(8) . .
O3 Ho2 O1 Te1 130.8(5) 1_655 .
O7 Ho2 O1 Te1 57.5(5) 1_665 .
O8 Ho2 O1 Te1 -18.2(5) . .
O9 Ho2 O1 Te1 -161.7(6) 1_655 .
Ho1 Ho2 O1 Te1 153.8(7) 1_655 .
O11 Ho2 O1 Ho1 112.7(3) . 1_655
O12 Ho2 O1 Ho1 26.2(4) . 1_655
O10 Ho2 O1 Ho1 -141.1(4) . 1_655
O3 Ho2 O1 Ho1 -22.9(2) 1_655 1_655
O7 Ho2 O1 Ho1 -96.3(3) 1_665 1_655
O8 Ho2 O1 Ho1 -172.0(3) . 1_655
O9 Ho2 O1 Ho1 44.5(2) 1_655 1_655
O3 Te1 O2 Ho1 -121.9(5) . 2_656
O1 Te1 O2 Ho1 143.7(5) . 2_656
Ho1 Te1 O2 Ho1 132.7(6) 1_655 2_656
Ho1 Te1 O2 Ho1 -97.8(5) . 2_656
O3 Te1 O2 Ho1 105.4(2) . 1_655
O1 Te1 O2 Ho1 11.0(2) . 1_655
Ho1 Te1 O2 Ho1 129.5(2) . 1_655
O1 Te1 O3 Ho1 129.6(3) . .
O2 Te1 O3 Ho1 40.9(3) . .
Ho1 Te1 O3 Ho1 88.8(2) 1_655 .
O1 Te1 O3 Ho2 -94.1(3) . 1_455
O2 Te1 O3 Ho2 177.3(3) . 1_455
Ho1 Te1 O3 Ho2 -134.9(3) 1_655 1_455
Ho1 Te1 O3 Ho2 136.3(5) . 1_455
O2 Ho1 O3 Te1 -9.7(4) 2_656 .
O6 Ho1 O3 Te1 -153.3(3) . .
O1 Ho1 O3 Te1 124.6(3) 1_455 .
O5 Ho1 O3 Te1 -86.4(3) . .
O4 Ho1 O3 Te1 40.0(3) . .
O9 Ho1 O3 Te1 -162.0(3) . .
O2 Ho1 O3 Te1 90.5(3) 1_455 .
Te1 Ho1 O3 Te1 104.6(3) 1_455 .
Ho2 Ho1 O3 Te1 146.4(4) 1_455 .
Ho1 Ho1 O3 Te1 44.5(4) 2_556 .
O2 Ho1 O3 Ho2 -156.1(2) 2_656 1_455
O6 Ho1 O3 Ho2 60.3(4) . 1_455
O1 Ho1 O3 Ho2 -21.7(2) 1_455 1_455
O5 Ho1 O3 Ho2 127.2(2) . 1_455
O4 Ho1 O3 Ho2 -106.3(2) . 1_455
O9 Ho1 O3 Ho2 51.6(2) . 1_455
O2 Ho1 O3 Ho2 -55.9(3) 1_455 1_455
Te1 Ho1 O3 Ho2 -41.76(18) 1_455 1_455
Te1 Ho1 O3 Ho2 -146.4(4) . 1_455
Ho1 Ho1 O3 Ho2 -101.9(2) 2_556 1_455
O2 Ho1 O4 S1 -8.1(4) 2_656 2_656
O6 Ho1 O4 S1 43.8(7) . 2_656
O1 Ho1 O4 S1 136.7(5) 1_455 2_656
O5 Ho1 O4 S1 -77.1(5) . 2_656
O3 Ho1 O4 S1 -150.2(5) . 2_656
O9 Ho1 O4 S1 -177.8(4) . 2_656
O2 Ho1 O4 S1 69.7(5) 1_455 2_656
Te1 Ho1 O4 S1 104.8(5) 1_455 2_656
Te1 Ho1 O4 S1 -127.9(5) . 2_656
Ho2 Ho1 O4 S1 172.3(5) 1_455 2_656
Ho1 Ho1 O4 S1 32.8(4) 2_556 2_656
O6 S1 O5 Ho1 -94.1(6) 1_655 .
O7 S1 O5 Ho1 144.7(5) . .
O4 S1 O5 Ho1 26.3(7) 2_656 .
O2 Ho1 O5 S1 -45.4(6) 2_656 .
O6 Ho1 O5 S1 -129.6(6) . .
O1 Ho1 O5 S1 137.3(5) 1_455 .
O3 Ho1 O5 S1 84.9(6) . .
O4 Ho1 O5 S1 20.2(7) . .
O9 Ho1 O5 S1 151.3(6) . .
O2 Ho1 O5 S1 -90.8(6) 1_455 .
Te1 Ho1 O5 S1 -168.7(2) 1_455 .
Te1 Ho1 O5 S1 57.4(6) . .
Ho2 Ho1 O5 S1 117.2(5) 1_455 .
Ho1 Ho1 O5 S1 -62.6(6) 2_556 .
O2 Ho1 O6 S1 52.9(5) 2_656 1_455
O1 Ho1 O6 S1 -82.9(6) 1_455 1_455
O5 Ho1 O6 S1 135.7(6) . 1_455
O3 Ho1 O6 S1 -154.8(4) . 1_455
O4 Ho1 O6 S1 3.0(8) . 1_455
O9 Ho1 O6 S1 -146.6(6) . 1_455
O2 Ho1 O6 S1 -22.8(5) 1_455 1_455
Te1 Ho1 O6 S1 -51.5(5) 1_455 1_455
Te1 Ho1 O6 S1 160.2(2) . 1_455
Ho2 Ho1 O6 S1 -117.4(5) 1_455 1_455
Ho1 Ho1 O6 S1 13.7(5) 2_556 1_455
O6 S1 O7 Ho2 -78.2(6) 1_655 1_445
O5 S1 O7 Ho2 43.7(7) . 1_445
O4 S1 O7 Ho2 162.1(5) 2_656 1_445
O2 Ho1 O9 Ho2 -171.9(3) 2_656 1_455
O6 Ho1 O9 Ho2 143.7(2) . 1_455
O1 Ho1 O9 Ho2 35.90(17) 1_455 1_455
O5 Ho1 O9 Ho2 -134.9(2) . 1_455
O3 Ho1 O9 Ho2 -41.68(17) . 1_455
O4 Ho1 O9 Ho2 -13.2(3) . 1_455
O2 Ho1 O9 Ho2 79.2(2) 1_455 1_455
Te1 Ho1 O9 Ho2 52.44(13) 1_455 1_455
Te1 Ho1 O9 Ho2 -49.85(13) . 1_455
Ho1 Ho1 O9 Ho2 107.8(2) 2_556 1_455
O13 S2 O10 Ho2 104.3(8) . .
O12 S2 O10 Ho2 -134.4(8) 2_865 .
O11 S2 O10 Ho2 -15.6(9) 2_765 .
O1 Ho2 O10 S2 -60.6(10) . .
O11 Ho2 O10 S2 46.1(8) . .
O12 Ho2 O10 S2 128.7(8) . .
O3 Ho2 O10 S2 -164.8(7) 1_655 .
O7 Ho2 O10 S2 -106.4(8) 1_665 .
O8 Ho2 O10 S2 -30.3(8) . .
O9 Ho2 O10 S2 110.4(8) 1_655 .
Ho1 Ho2 O10 S2 -149.6(5) 1_655 .
O1 Ho2 O11 S2 45.3(8) . 2_765
O12 Ho2 O11 S2 -179.9(8) . 2_765
O10 Ho2 O11 S2 -105.5(8) . 2_765
O3 Ho2 O11 S2 112.7(8) 1_655 2_765
O7 Ho2 O11 S2 -37.3(11) 1_665 2_765
O8 Ho2 O11 S2 -27.3(8) . 2_765
O9 Ho2 O11 S2 106.1(8) 1_655 2_765
Ho1 Ho2 O11 S2 80.7(8) 1_655 2_765
O1 Ho2 O12 S2 172.1(10) . 2_865
O11 Ho2 O12 S2 80.7(12) . 2_865
O10 Ho2 O12 S2 -14.6(11) . 2_865
O3 Ho2 O12 S2 -141.4(12) 1_655 2_865
O7 Ho2 O12 S2 -79.8(12) 1_665 2_865
O8 Ho2 O12 S2 25.4(14) . 2_865
O9 Ho2 O12 S2 154.8(12) 1_655 2_865
Ho1 Ho2 O12 S2 -172.4(11) 1_655 2_865
